Abstract
The interfacial stress in a carbon fiberreinforced polymer (CFRP) plate for strengthening the top flange of a boxgirder bridge was theoretically investigated. According to the force analysis results of the boxgirder structure, the most unfavorable force area was selected for modeling analysis. Using the simplified beam model, a CFRP plateconcrete interfacialstress calculation model was derived, and the closedform solution of the calculation model was obtained. Equivalent simplified test specimens were designed according to the boxgirder structure to verify the reliability of the theoretical model. Then, fourpoint bending tests of the sample were performed. In these tests, the debonding failure modes and strain in the CFRP plate were examined. The CFRP plateconcrete interfacial stress was calculated according to the strain data of the CFRP plate in the experimental tests. Then compared the experimental results with the theoretical results. Furthermore, the corresponding interfacial stresses were calculated and compared according to the different load levels specified in the code. A series of theoretical and experimental comparisons were performed to verify the reliability of the proposed CFRPconcrete interfacial stress closedform solution model.
Keywords:
CFRP plate; strengthened box girder; debonding failure; interfacial stresses; theoretical model; bridge
Graphical Abstract
Keywords:
CFRP plate; strengthened box girder; debonding failure; interfacial stresses; theoretical model; bridge
1 INTRODUCTION
Carbon fiberreinforced polymer (CFRP) is generally formed through a series of heat treatments, and carbon fiber tow and epoxy resin are typically used as basic materials. Kromoser et al. (2019B. Kromoser, P. Preinstorfer, J. Kollegger. (2019) Building lightweight structures with carbon fiberreinforced polymerreinforced ultrahighperformance concrete. fib. International Federation for Structural Concrete 20: 730744.) introduced CFRP as a lightweight and highstrength material whose density and tensile strength are approximately 20% of and five times those of steel, respectively; the CFRP plate shape is shown in Figure 1(a). Burgoyne (2004C.J. Burgoyne. (2004) Does FRP have an economic future? Advanced Composite Materials in Bridges and Structures, Calgary, Alberta, July 2023.) reported that because of its excellent material properties, CFRP has been used to enhance the durability of reinforced concrete structures. Compared with the traditional bridgestrengthening methods, the application of CFRP materials can significantly reduce the dead weight and impact on the bridge structure. Czaderski & Motavalli (2007C. Czaderski, M. Motavalli. (2007) 40Yearold fullscale concrete bridge girder strengthened with prestressed CFRP plates anchored using gradient method. Composites Part B 38: 878886.) used a prestressed CFRP plate to strengthen an old concrete bridge and employed the gradient method to anchor the plate. Hosseini et al. (2009A. Hosseini, E. Ghafoori, R. AlMahaidi, XL. Zhao, M. Motavalli. (2009) Strengthening of a 19thcentury roadway metallic bridge using nonprestressed bonded and prestressed Unbonded CFRP plates. Construction and Building Materials 209: 240  259.) performed a series of truckloading tests on a nonprestressed CFRPstrengthened metallic bridge and concluded that the tensile stresses were reduced via strengthening. Gallego et al. (2017J.M. Gallego, J. Michels, C. Czaderski. (2017) Influence of the asphalt pavement on the shortterm static strength and longterm behaviour of RC slabs strengthened with externally bonded CFRP strips. Engineering Structures 150: 481496., 2018) studied the lateral bending performance of a concrete boxgirder bridge and proposed the use of a CFRP board to strengthen the boxgirder cantilever.
Different types of cracks appear in concrete boxgirder bridges when they are subjected to various loads and exposed to harsh environments. In this regard, the use of the CFRP plate can improve the lateral rigidity of the girder. The commonly adopted method involves pasting a CFRP plate of a certain length on the top edge of the concrete box girder, as shown in Figure 1(b). In the negativeflexural moment zone, the CFRP plate can maintain the tensile force by functioning similar to that of tensile steel bars. However, the debonding failure of the CFRP plate usually occurs at the end of the concrete structure reinforced by the CFRP plate, as shown in Figure 1(b).
Lu et al. (2005X.Z. Lu, L.P. Ye, J.G. Teng, J.J. Jiang. (2005) Mesoscale finite element model for FRP sheets/plates bonded to concrete. Engineering Structures 27: 564575.) and Smith & Teng (2002S.T. Smith, J.G. Teng. (2002) FRPstrengthen RC beams. I: review of debonding strengthen models. Engineering Structure24(4): 385395.) investigated the main cause of the CFRP plateend debonding failure and found that the interfacial stress between the CFRP and the concrete was larger than the ultimate bearing capacity of the concrete. Sun et al. (2017aW. Sun, X. Peng, H.F. Liu, H.P. Qi. (2017a) Numerical studies on the entire debonding propagation process of FRP strips externally bonded to the concrete substrate. Construction and Building Materials 149: 218235., 2017b) simulated the entire debonding failure process of a CFRP plate on a concrete structure and proposed a bifold line interfacial bonding model based on finiteelement analysis results. Ferrier et al. (2011E. Ferrier, L. Michel, B. Jurkiewiez, P. Hamelin. (2011) Creep behaviour of adhesives used for external FRP strengthening of RC structures. Construction and Building Materials,25: 461467., 2016) and Ferrier and Agbossou (2017) performed a series of experimental studies on FRP concrete doubleshear specimens (test temperature range of 40 to 20 °C). The interface characteristics of CFRP concrete after special process treatment at a certain temperature were analyzed using a highorder fracture mechanics model. Wang & Petrů (2019X.M. Wang, M. Petrů. (2019) Mode I fracture evaluation of CFRPtoconcrete interfaces subject to aggressive environments agents: Freezethaw cycles, acid, and alkaline solution. Composites Part B 168: 58188.) experimentally investigated the mechanical behavior of the CFRPconcrete interface after freezethaw cycling. The results indicated that the failure mode was affected by the freezethaw cycling; as the number of cycles increased, the failure mode changed from tensile failure to interface failure.
In this study, the top flange of a boxgirder bridge was strengthened using a CFRP plate to investigate the facile occurrence of plateend debonding failure. Using the force analysis results of the box girder, according to the debonding failure of the plate end of the CFRPconcrete interface, a closedform theoretical calculation model for the interfacial stress was proposed. Beam specimens were designed according to the equivalent simplification of the box girder. A fourpoint flexural test was performed on the test beams, and the reliability of the proposed calculation model was verified by comparing experimental results with theoretical results.
In this paper, a calculation method for the higherorder analytical solutions of interfacial stress to avoid the closedform approximate solution of a simply supported beam is presented. Moreover, different loading situations, including a flexural moment, uniform load, and concentrated load, are simultaneously considered in the proposed calculation model. One of the advantages of the model is that it derives the expression of the solution in a closed form. Moreover, in the thickness direction of the adhesive layer, the longitudinal stress variation of the interfacial stress is considered.
2 THEORETICAL MODEAL OF INTEEFACIAL STRESS
2.1 Analysis model
Lateral force analysis of the box girder is performed according to the actual loading condition of the bridge structure shown in Figure 2(a). According to the mechanical analysis results, the maximum negative flexural moment exists on one side of the boxgirder roof. Thus, this part of the boxgirder roof is selected for the analysis; the simplified beam model is shown in Figure 2(b). Considering that the boxgirder web has a certain thickness, it can be simplified as a support for the boxgirder roof. The dead weight of the asphalt pavement on the bridge deck is regarded as a uniform load (q). To simulate the actual forces on the structure, flexural moments and concentrated loads are applied to the simplified model.
To facilitate its use in actual engineering, the simplified beam model is subjected to further equivalent transformation (Figure 2(b)). In the equivalent simply supported beam model shown in Figure 2(c), a coordinate system wherein the origin is the intersection of the boxgirder web and roof is established. The plane where the top flange is regarded as the Xaxis, and the positive direction of the Yaxis points to the bottom plate of the box girder. In this equivalent calculation model, the CFRP plate originally placed on the top flange of the box girder is transferred to the bottom of the beam model. The lengths of the beam and CFRP plate are 2L and 2l, respectively.
According to the principle of equivalent force, the original simple support located at the midspan is converted into concentrated loads and placed at the beam ends. After the conversion, an equivalent simply supported beam model with traditional simple support boundary conditions is obtained. The original reaction forces of the midspan support are converted into two new concentrated forces (P), which are loaded on the both sides of the midspan position of the beam model. Moreover, the concentrated load originally located at the beam end, as shown in Figure 2(b), is converted into a simple support, as shown in Figure 2(c). According to the force analysis results, the actual force in the beam remains unchanged before and after the transition at the boundary condition.
2.2 Basic assumptions
The theoretical model is subjected to a flexural moment (M), concentrated load (P), and uniform load (q). In the interfacial stress analysis of this model, the following basic assumptions are made.

The beam model is divided into several layers, each of which is considered as linearly elastic. The anisotropy of the material is ignored, and the material is considered to be homogeneous.

The deformation of adjacent layers at their interface is ignored; i.e., it is assumed that there is no relative slip at the CFRPconcrete interface.

The CFRP plate and concrete beam in the model follow the Euler beam theory, and the adhesive layer conforms to the plane stressstrain criterion.

The thinplate flexural theory is used for the CFRP platereinforced concrete beam.

The longitudinal stress in the thickness direction of the adhesive layer is assumed to change linearly.

For a beam with debonding failure, the shear deformation is presumed to cause the anisotropy of the layers at the interface in the longitudinal section of the beam.
2.3 Boundary conditions
For modeling convenience, the concrete beams, bonding layers, and CFRP plates are labeled with the numbers 13, as shown in Figure 3(a). Similarly, each interface layer is marked with a number ranging from (0) to (3). For the beam model cross section (Figure 3(b)), the width of each interface layer is marked as b(i), where i is the number of the interface layer. Moreover, the width of the adhesive layer is considered to be identical to that of the CFRP plate, i.e., b(0) = b(1) = b(2).
Each layer is separately analyzed according to the established coordinate system in the overall beam model. A local coordinate system can be established at the geometric center of different layers, as shown in Figure 3(c). The force condition of selected beam microsegments based on which the forcebalance equations below are established is presented in Figure 3(c).
Axialforce equilibrium:
Shearforce equilibrium:
Moment equilibrium:
The definitions of the symbols in the foregoing equations are presented in Table 1.
Attentionally,
The following equations can be established according to the boundary conditions shown in Figure 3(c):
where
2.4 Analytical solution
For the CFRP plateadhesive interface (i = 1) and the adhesiveconcrete interface (i = 2), the interfacial stress can be calculated using the Fourier series expansion equations. The normal and shear stresses in the i^{th} layer can be expressed as follows:
By substituting Eq. (3) in Eq. (1), the following equations can be derived:
where
For the adhesive layer, considering assumptions (3) and (5), the following equations may be satisfied:
where
Then, the following equations can be obtained.
In the foregoing,
Moreover, the following relationships can be obtained:
where
By substituting Eqs. (4)(8) in Eq. (3), all the variables in Eq. 3except for
According to the principle of the variational method, the following equations can be obtained from Eq. (9):
where the parameters
To further simplify Eq. (10),
Here,
Hence, the closedform solution of the interfacial stress can be obtained, and the equations can be expressed as follows:
Here,
where
3 INTERFACIAL STRESS TESTS OF CFRPCONCRETE SPECIMENS
The theoretical model of the proposed CFRPreinforced concrete beams was experimentally verified. The beam specimen was designed according to the boxgirder force analysis results, and the test setup and instrumentation were based on the actual bridge load boundary conditions.
3.1 Experimental specimens and test setup
3.1.1 Specimen description
According to the analysis results of the original bridge structure (Figure 2(a)), a CFRPstrengthened concrete beamslab specimen was designed. The test specimen had a reinforced concrete beamslab structure with a rectangular crosssection. Its dimensions were l × b × h = 4000 mm × 650 mm × 280 mm. The concrete grade of the test beam was C45, and the reinforcement in the tension and compression zones was HRB400 rebar with a diameter of 12 mm. The test beam reinforcement layout is shown in Figure 4.
To strengthen the test beam, three CFRP plates with a certain length were pasted on its top surface, as shown in Figure 5(a). The crosssectional size of the CFRP plate was h × b = 1.4 mm × 100 mm. After the test beam was reinforced with the CFRP plate, its top surface was paved with stone mastic asphalt to simulate the hightemperature effect and dead weight of the asphalt layer, as shown in Figure 5(b).
In the test, two sets of specimens (a total of four specimens) were investigated. The FDBL series, which had one test beam, was used for comparison. The FX series contained three test beams (i.e., FX1, FX2, and FX3) whose specimens were strengthened with CFRP plates. The strengthening scheme is shown in Figure 5(a).
3.1.2 Material property
For this test, the materials used in the test beam mainly included the CFRP plate, concrete, steel bars, and adhesives. The elastic moduli of the C45 concrete and steel bars were 33.5 and 2.52.6 GPa, respectively. The main performance parameters of the CFRP plate and adhesive are presented in Table 2.
3.1.3 Test procedure and instrumentation
The beam specimens were simply supported at the midspan of the test beam. Two bearings were arranged at 400 mm on both sides of the beam midspan, and the loading positions were at the two ends of the beam. Moreover, displacement meters were arranged at the beam ends and midspan positions to measure the beam deformation during the test. The test setup is shown in Figures 6(a) and (b).
The interfacial stress between the CFRP plate and the concrete was the focus of this study; hence, it was necessary to examine the strain distribution at the CFRPconcrete interface. However, measuring the strain at the interface layer during the test is difficult. It can be calculated through a certain equivalent transformation of the CFRPplate strain. To measure the strain, a part of the asphalt layer was removed before the test. Considering the symmetry of the structure, a halfbeamlong portion of the asphalt layer was removed from each of the CFRP plates. Strain gauges were arranged on the outer layers of the three CFRP plates; the layout of these gauges on the CFRP plate is shown in Figure 6(c).
A steel bearing plate was arranged at each loading position to prevent stress concentration. A vertical force of 300 kN was simultaneously applied to each steel bearing plate. During the loading process, the load was gradually applied for preventing the excessive deformation of the specimen, as shown in Figure 6(d).
3.2 Failure characteristics and observations
3.2.1 Debonding failure phenomenon and bearing capacity
The failure form and bearing capacity of the specimen were investigated during the test. The common failure modes of CFRPstrengthened concrete beams are as follows.

a) Plateend debonding failure: when the interfacial stress at the end of the CFRP plate exceeds the ultimate bearing capacity of the material, plateend interfacial debonding failure is expected to occur. Thus, this type of failure mode is usually caused by high interfacial stress.

b) Intermediate crackinduced debonding: various flexural cracks and flexureshear cracks typically appear at the midspan of the beam. Usually, intermediate cracks lead to this type of failure mode.
The failure patterns of different specimens were examined during the test, as shown in Figure 7.
As shown in Figure 7, the failure mode of the FDBL specimen was mainly the ductile deformation of the tensile steel bar, and those of the FX series specimens were concrete cracking in the negativeflexural moment zone and debonding failure of the CFRP plate.
For specimen FX1, distinct intermediate crackinduced debonding failure and plateend debonding failure were observed. After the beam was unloaded, the CFRP plate of the test beam exhibited a significant cumulative deformation, and a void phenomenon occurred between the CFRP plate and the concrete at the midspan.
The failure mode of specimen FX2 was similar to that of specimen FX1. However, the debonding failure of specimen FX2 was interfacial debonding failure between the CFRP plate and adhesive layer, whereas that of specimen FX1 was the debonding failure of the surface layer concrete cover around the interface layer.
The debonding failure of specimen FX3 was not observed at the midspan of the test beam and only occurred at the plate end.
Compared with the plastic deformation of specimen FX1, those of FX2 and FX3 were smaller. This may have been due to problems in the construction quality during the pasting process and the hightemperature effect during asphalt paving. The foregoing also resulted in debonding failure or voiding at some positions of the interface layer before the test. This preexisting debonding failure prevented the full exertion of the tensile effect of the CFRP plate.
For comparison, the moments in the specimens at different loading stages were calculated. The calculation results and debonding patterns are presented in Table 3.
As indicated by Table 2, the average ultimate bearing capacity of the strengthened specimen was 66.7% higher than that of the unstrengthened specimen. It can be concluded that the CFRPstrengthened method can effectively improve the ultimate bearing capacity and delay the occurrence of debonding failure.
3.2.2 CFRPplate strain
The strain distributions in the CFRP plates under different loads were measured using the strain gauges on the CFRP plates. The strain distributions in the different specimens are shown in Figure 8.
As shown in Figure 8, the strain change in the CFRP plate was not distinct when the loading level was low. As the loading level increased, the strain distribution in the CFRP plate exhibited nonlinearity. When the loading level was high, the CFRP plates exhibited high and low strain values at the midspan and end positions of the plates, respectively. When the loading level was approximately 220 kN, the CFRP strain 1400 mm from the plate end exceeded that at the adjacent position. The expansion of cracks in the concrete beam was the main reason for this situation. Near the midspan, a highconcrete stress area existed around the crack position. The CFRPplate strain was also increased by the bonding force between the CFRP plate and the concrete.
3.2.3 Interfacial shear stress between CFRP plate and concrete
Rahimi et al. (2001H. Rahimi, A. Hutchinson. (2001) Concrete beams strengthened with externally bonded FRP plates. Journal of Composites for Construction 5(1):4456.) proposed a method based on force balance for calculating the shear stress of the CFRP platereinforced concrete structure interface, and the interfacial stress between the CFRP plate and the concrete can be determined using the adjacent strain value in the CFRP plate.
The interfacial stress can be calculated using the strain values measured by the adjacent strain gauges, via the following equation.
Assume that the adjacent strain values in the CFRP plate are
where
The interfacial shear force between the CFRP plate and the concrete can be calculated using the following equation:
where
According to the principle of force balance,
where the obtained interfacial shear stress (
Rahimi et al. (2001H. Rahimi, A. Hutchinson. (2001) Concrete beams strengthened with externally bonded FRP plates. Journal of Composites for Construction 5(1):4456.) proposed a calculation method for the shear stress at the interface between the CFRP plate and the concrete. The calculation results for the interfacial shear stress of each specimen are shown in Figure 9.
Considering that the bonding strength of the adhesive layer is high, the interfacial debonding failure between the CFRP plate and concrete is generally indicated by the debonding failure of the concrete surface layer. It can be considered that interfacial debonding failure has occurred when the interfacial shear stress exceeds the concrete tensile strength. Therefore, the calculated interfacial shear stress was compared with the concrete ultimate bearing capacity in tension, as shown in Figure 9. When the loading level was low, the interfacial shear stress was relatively low. The interfacial shear stress fluctuated as the load increased, but it did not reach the tensile strength of concrete materials.
For specimens FX2 and FX3, the position where the interface shear stress curve changed suddenly was at the end of the CFRP plate, and the interfacial shear stress exceeded the concrete bearing capacity in tension. It is considered that plateend debonding failure occurred at this position in the CFRP plate, corresponding to the failure mode of the specimen during the test (Figures 7(b)(d)).
However, for specimen FX1, the interfacial shear stress at the end of the CFRP plate fluctuated only slightly under the different loading levels. Considering the failure form of the specimen shown in Figure 7(a), a large plastic deflection was observed after the loading process. The CFRP plate was considered to be not fully effective, and voiding of the interface layer may have existed before the test. The CFRP plate of specimen FX1 was in the free end state during the test. Therefore, no distinct deformation occurred in this part of the CFRP plate, and the interfacial shear stress in this segment could not be accurately measured.
4 ANALYSIS OF RESULTS AND APPLICATIONS
4.1 Comparison between analysis and test results
The interfacial stresses calculated using the theoretical model and measured in the flexural beam tests are compared in Figure 10.
As shown, the distribution of the experimental values agreed well with the theoretical curve, indicating that the proposed interfacialstress calculation model is reliable.
Similar to the test results, the shear stress of the CFRPconcrete interface at the end of the CFRP plate changed significantly near the end position. The difference between the calculation and test rests for the end position was small.
The peak of the interface normal stress in the CFRP plateconcrete interface appeared at the end position. The interface layer at this position was subject to tensile stress and prone to debonding failure.
Along the longitudinal direction of the CFRP plate, the interfacial normal stress rapidly decreased from the end position and became negative. At this position, the interface was under pressure, preventing debonding failure. The interface normal stress approached zero with the increasing distance from the end of the CFRP plate.
4.2 Application to structural calculation
According to the general codes for the design of highway bridges and culverts adopted in China, two types of vehicleload grades are employed in bridge design: highway classes I and II. Lane loading can be converted into a uniform load (qk) and concentrated force (pk). When the load grade is highway class I, the standard value of the uniform load is 10.5 kN/m, and that of the concentrated force is based on the bridge span. When the calculation span is <5 m and >50 m, the load is considered to be 270 and 360 kN, respectively. For other spans, the linearinterpolation method is employed to obtain the load value. When the vehicleload grade is highway level II, the lane loading magnitude adopted is 0.75 times that specified for highway class I.
Accordingly, the lane loading in the general specifications was converted into the load of the CFRP plate reinforced boxgirder roof in this study. The maximum and minimum values of the concentrated load specified by the lane loading of highway classes I and II were selected for the calculation. The calculation results for the interfacial stress distributions under different loading levels are shown in Figure 11.
As shown in Figure 11 (a) and (b), under different loads (highway class IP= 270kN, IP= 360kN, IIP= 202.5kN, IIP= 270kN), the interface normal stress and shear stress appear peak near the end of CFRP plate peeling, and the interface normal stress and shear stress near the end of CFRP plate peeling approach to zero at the end of CFRP plate peeling. The variation range of the shear stress curve data on the peak value is relatively significant compared with that of the normal stress data, and the peak value of the normal stress curve data only fluctuates within a small range. The comparison of the peak value is shown in Table 4.
At the same time, it can be seen from Figure (a) and (b) that under four different loads (highway class IP= 270kN, IP= 360kN, IIP= 202.5kN, IIP= 270kN), for shear stress and normal stress in Figure (a), the overall fluctuation trend of the four curves in each figure is similar. To further scientific analysis of the phenomenon, we with no significant difference between every four sets of data for the assumptions, the significance level of 0.01 a, respectively according to the theory of shear stress and normal stress of the four groups of data analysis of variance, can draw the following conclusions: (1) for shear stress data by variance analysis, the parameter values of Pvalue is 0.97, the parameter value F 0.09, parameter value F crit is 3.9. (2) for normal stress data by variance analysis, the pvalue of the parameter is 0.99, the parameter value F is 0.003, and the parameter value F crit is 3.8, as shown in Tables 5 and 6.
Analysis of variance of theoretical interface normal stress data under different highway grades.
Through the comparison of these parameters, the relationship can be obtained: Pvalue > a, F < F crit. According to the ANOVA evaluation criteria, the null hypothesis can be accepted and no significant difference can be found between every four groups of data under different stresses. Therefore, in each graph, the overall fluctuation trend of the four curves is similar and the range of change is not large. According to the above analysis, the distribution characteristics of the model are relatively stable and can be applied to engineering practice.
5 CONCLUSIONS
A closed interfacialstress calculation model was developed by studying the interfacial stress between a CFRP plate and concrete and the load characteristics of the bridge. To verify the reliability of the theoretical model, experimental tests were performed. According to the results, the following conclusions are drawn.

With the higherorder analytical solutions of the interfacialstress calculation model, the approximation used in the previous solution of the simply supported beam is avoided.

The concentrated load, uniform load, and flexural moment were considered in the proposed model. Different loading conditions can improve the usefulness of theoretical models in practical engineering.

The test beams were designed according to the box girder. The intermediate cracking debonding failure and plateend debonding failure of the test beam can be observed. The interfacial shear stress was obtained according to the adjacent strain in the CFRP plate, and the highinterfacial stress region coincided with the occurrence of the debonding phenomenon in the test beams.

The interfacial stress obtained via the flexural tests agreed well with the calculation results of the theoretical model, hence validating the theoretical model.

The interfacialstress curve calculated using the theoretical model according to the different loading levels specified in the code was consistent with the interfacialstress curve obtained from the test.

The change response sensitivity of the interfacial shear stress was higher than that of the interfacial normal stress under different loading levels and according to ANOVA, the overall fluctuation trend of the four curves in each graph is similar, and the range of change is small. The distribution characteristics of the model are relatively stable and can be applied to engineering practice
ACKONWLEDGEMENTS
This work was financially supported by the Brand Professional Funding Project of Jiangsu Province (Grant No. PPZY2015B143), the National Natural Science Foundation of China (Grant No. 51508368), the Science and Technology Project of Housing and UrbanRural Development Department of Jiangsu Province(Grant No.2019ZD010), the Postgraduate Research & Practice Innovation Program of Jiangsu Province (Grant No. SJCX18_0879), and Key Project of Innovation and Entrepreneurship of College students in Jiangsu Province (Grant No. 201810332019Z).
REFERENCES
 A. Hosseini, E. Ghafoori, R. AlMahaidi, XL. Zhao, M. Motavalli. (2009) Strengthening of a 19thcentury roadway metallic bridge using nonprestressed bonded and prestressed Unbonded CFRP plates. Construction and Building Materials 209: 240  259.
 B. Kromoser, P. Preinstorfer, J. Kollegger. (2019) Building lightweight structures with carbon fiberreinforced polymerreinforced ultrahighperformance concrete. fib. International Federation for Structural Concrete 20: 730744.
 C.J. Burgoyne. (2004) Does FRP have an economic future? Advanced Composite Materials in Bridges and Structures, Calgary, Alberta, July 2023.
 C. Czaderski, M. Motavalli. (2007) 40Yearold fullscale concrete bridge girder strengthened with prestressed CFRP plates anchored using gradient method. Composites Part B 38: 878886.
 H. Rahimi, A. Hutchinson. (2001) Concrete beams strengthened with externally bonded FRP plates. Journal of Composites for Construction 5(1):4456.
 J.M. Gallego, J. Michels, C. Czaderski. (2017) Influence of the asphalt pavement on the shortterm static strength and longterm behaviour of RC slabs strengthened with externally bonded CFRP strips. Engineering Structures 150: 481496.
 J.M. Gallego, C. Czaderski, M. Breveglieri, J. Michels. (2018)Fatigue behaviour at elevated temperature of RC slabs strengthened with EB CFRP strips. Composites Part B 141: 3749.
 X.Z. Lu, L.P. Ye, J.G. Teng, J.J. Jiang. (2005) Mesoscale finite element model for FRP sheets/plates bonded to concrete. Engineering Structures 27: 564575.
 S.T. Smith, J.G. Teng. (2002) FRPstrengthen RC beams. I: review of debonding strengthen models. Engineering Structure24(4): 385395.
 W. Sun, X. Peng, H.F. Liu, H.P. Qi. (2017a) Numerical studies on the entire debonding propagation process of FRP strips externally bonded to the concrete substrate. Construction and Building Materials 149: 218235.
 W. Sun, X. Peng, Y. Yu. (2017b) Development of a simplified bond model used for simulating FRP strips bonded to concrete. Composite Structures 171: 462472.
 E. Ferrier, L. Michel, B. Jurkiewiez, P. Hamelin. (2011) Creep behaviour of adhesives used for external FRP strengthening of RC structures. Construction and Building Materials,25: 461467.
 E. Ferrier, O. Rabinovitch, L. Michel. (2016) Mechanical behavior of concreteresin adhesive FRP structural assemblies under low and high temperatures. Construction and Building Materials, 127: 10171028.
 E. Ferrier, A. Agbossou. (2017) Temperature effects on the shear capacity of external bonded fiber reinforced polymer on concrete. Construction and Building Materials 152: 333344.
 X.M. Wang, M. Petrů. (2019) Mode I fracture evaluation of CFRPtoconcrete interfaces subject to aggressive environments agents: Freezethaw cycles, acid, and alkaline solution. Composites Part B 168: 58188.
 H. Rahimi, A. Hutchinson. (2001) Concrete beams strengthened with externally bonded FRP plates. Journal of Composites for Construction 5(1):4456.
Publication Dates

Publication in this collection
03 May 2021 
Date of issue
2021
History

Received
22 Sept 2020 
Reviewed
22 Mar 2021 
Accepted
24 Mar 2021 
Published
29 Mar 2021